Local Magnetoelectric Effect in La-Doped BiFeO3 Multiferroic Thin Films Revealed by Magnetic-Field-Assisted Scanning Probe Microscopy
© The Author(s). 2016
Received: 14 April 2016
Accepted: 24 June 2016
Published: 30 June 2016
Multiferroic La-doped BiFeO3 thin films have been prepared by a sol-gel plus spin-coating process, and the local magnetoelectric coupling effect has been investigated by the magnetic-field-assisted scanning probe microscopy connected with a ferroelectric analyzer. The local ferroelectric polarization response to external magnetic fields is observed and a so-called optimized magnetic field of ~40 Oe is obtained, at which the ferroelectric polarization reaches the maximum. Moreover, we carry out the magnetic-field-dependent surface conductivity measurements and illustrate the origin of local magnetoresistance in the La-doped BiFeO3 thin films, which is closely related to the local ferroelectric polarization response to external magnetic fields. This work not only provides a useful technique to characterize the local magnetoelectric coupling for a wide range of multiferroic materials but also is significant for deeply understanding the local multiferroic behaviors in the BiFeO3-based systems.
Multiferroic materials refer to a class of materials which possess the intrinsic coupling of two or more ferroic orders (e.g., ferroelectricity, ferroelasticity, and ferromagnetism) [1, 2]. Among them, magnetoelectric materials exhibiting both ferroelectric and ferromagnetic characteristics have received much attention due to their great potential in multifunctional applications such as spintronics, memory, and sensors [3–5]. The magnetoelectric coupling between two order parameters makes it possible to manipulate the polarization states by external magnetic fields  or vice versa [7, 8]. In single-phase multiferroic materials reported by now, BiFeO3 (BFO, with a perovskite ABO3 structure)  is an ideal candidate which shows unambiguous room-temperature magnetoelectric coupling effect with a Curie temperature of 1103 K and a Néel temperature of 643 K.
In spite of such favorable features, the practical applications of BFO are still limited for several reasons such as formation of secondary phase during preparation, weak magnetoelectric coupling coefficients, and high leakage current . Fortunately, these drawbacks can be overcome by the epitaxial constraints or chemical doping. Suitable ionic doping in the A or B sites of BFO thin films has been widely accepted to improve their magnetic, electric, and magnetoelectric properties [11–14]. Introduction of rare earth ions, particularly La-doped BFO, has been demonstrated to exhibit favorable results . However, the local characterization of magnetoelectric coupling in such multiferroic thin films is still challenging and majority of previous works focus on the macroscopic magnetoelectric effect, while little attention has been paid to its microstructural evolution under either electric or magnetic fields [16, 17]. Besides, it is more important to characterize the local magnetoelectric coupling at nanoscale for practical applications such as high-density data-storage . The recently developed scanning probe microscope (SPM) techniques provide us an efficient way to study the local magnetoelectric coupling in multiferroic materials, accompanied with remarkable advantages in their non-invasive character, versatility, and high spatial resolution [19, 20].
In this work, by means of the magnetic-field-assisted scanning probe microscopy connected with an external ferroelectric tester, we systematically investigate the local magnetoelectric coupling behaviors in the multiferroic La-doped BiFeO3 polycrystalline thin films. The local ferroelectric polarization as well as the surface current distribution under external magnetic fields is observed. Based on the analysis about the change of average surface conductivity under various magnetic fields, we clarify the local magnetoelectric coupling process and the origin of local magnetoresistance in the La-doped BiFeO3 thin films, both of which are closely related to the local ferroelectric polarization response to external magnetic fields.
The Bi0.9La0.1FeO3 (BLFO) thin films were prepared on the commercial Pt/Ti/SiO2/Si (100) substrates by a typical sol-gel process and spin-coating technique. In detail, bismuth nitrate (Bi(NO3)3 · 5H2O), ferric nitrate (Fe(NO3)3 · 9H2O), and lanthanum nitrate (La(NO3)3 · 6H2O) were chosen as starting materials. Acetic acid and 2-methoxyethanol (1:4, volume ratio) were the solvent. The BLFO precursor solution was obtained by dissolving the nitrates into 2-methoxyethanol. Considering the loss of bismuth in the preparation process, 5 % excess Bi(NO3)3 · 5H2O was added. After being ultrasonic cleaned sequentially in deionized water, acetone, and ethanol, the Pt substrate was dried by N2. Then the precursor BLFO solution was spin-coated onto the substrate at 500 rpm for 8 s and 4000 rpm for 30 s in a glove box full of N2. Before coating the next layer, the film was dried at 200 °C for 5 min at a heating plate. The thickness of BLFO film was controlled by repeating times of the spin-coating procedure. Finally, the film was annealed at 550 °C for 10 min under oxygen atmosphere. The detailed preparation can also be found elsewhere .
Characterization and Measurements
The structural characteristic of the as-prepared BLFO film was carried out by the X-ray diffraction (XRD) analysis on a D/MAX-RA diffractometer with Cu Kα radiation. A scanning electron microscopy (SEM, ULTRA 55-44-08) was used to examine the cross-sectional morphology. The magnetization vs. magnetic field (M-H) hysteresis loop was measured using a superconducting quantum interference device (SQUID, Quantum Design). We used an atomic force microscopy (AFM) (NT-MDT Inc.) to characterize the surface topography, and the surface current distribution mapping was obtained by using the attached conductive-atomic force microscopy (c-AFM) with a Cr/Pt-coated tip. The tip which acted as a mobile top electrode was grounded, and the bias voltage was applied to the bottom electrode. The ferroelectric domain structures were revealed by piezoresponse force microscopy (PFM), and the external magnetic fields were generated by the Helmholtz coils from NT-MDT Inc. For local electrical measurements, tiny circular electrodes with the diameter of 20 μm were made by a conventional photolithography method . The local polarization vs. voltage (P-V) hysteresis loops were obtained by a standard ferroelectric analyzer (Precision Multiferroic, Radiant Inc.) connected to the AFM controller using a Signal Access Module (NT-MDT Inc.). The local I-V curve was measured by the single-point c-AFM mode. For comparison, macroscopic I-V measurements were also performed. Forty-nanometer Au electrodes were deposited onto the film using ion-sputtering technique through a shadow mask with the diameter of 0.2 mm, and the I-V curve was recorded by a Keithley 6517B electrometer. Without special descriptions, all the measurements were performed at room temperature and under ambient condition.
Results and Discussion
Basic Characterizations of the BLFO Thin Films
Figure 1c presents the typical surface AFM topographic image of the chosen 3 × 3 μm2 BLFO film. It can be observed that the as-prepared BLFO film is well-crystallized and the average grain size is about 100 nm. Besides, the film is rather dense and the average surface roughness is ~30 nm. Figure 1d gives the corresponding c-AFM mapping at a bias voltage of 6 V with the same area. It is easily concluded that the grain boundary is more conductive than the grain interior, which is consistent with our previous work . The local electrical conduction is attributed to the oxygen vacancies accumulated at the grain boundaries of polycrystalline BLFO film. We then performed the PFM measurements to test the local polarization response to external electric fields. The chosen 6 × 6 μm2 area was firstly written with +6 V bias voltage using a biased conductive tip; then, a central smaller square of 3 × 3 μm2 was reversely poled with −6 V bias voltage in the same way; finally, in the outer 10 × 10 μm2 area, both the PFM-phase and PFM-amplitude images were recorded under zero bias voltage, as depicted in Fig. 1e, f. Clearly, the BFLO film shows a switchable ferroelectric response to external electric fields, and the ferroelectric domains are altered to the opposite direction upon the application of reversed voltage. The above M-H and switchable PFM experimental results confirm the existence of both ferroelectricity and ferromagnetism in the present BLFO thin films.
Local Ferroelectric Polarization Behaviors Under External Magnetic Fields
Subsequently, we carried out the local P-V hysteresis loop measurements under various magnetic fields, as shown in Fig. 2d, e. All the tests were performed intentionally at 10 kHz to further exclude the influence of leakage current. With no magnetic field applied, a well-defined ferroelectric polarization hysteresis loop was obtained with a saturation polarization (P s) of ~18 μC/cm2. Upon the application of external magnetic fields, the P-V hysteresis loops emerge an obvious change with the external magnetic fields, indicative of evident magnetoelectric coupling in the BLFO thin film. The P s value increases sharply when the external magnetic field is applied from 0 to 40 Oe. However, when the external magnetic field is above 40 Oe, the P s value starts to decrease. Figure 2f gives the P s values derived from Fig. 2d, e as a function of external magnetic fields.
In general, the ferroelectric and magnetic characteristics in a BFO system are coming from two independent parts, i.e., the ferroelectric polarization is originated from the displacement of Bi3+ ions caused by the active 6 s2 loan pair while the magnetic property mainly comes from the Fe3+ ions and related cycloidal spin structures . The vectors of the ferroelectric polarization and antiferromagnetic spin are strongly coupled in a typical BFO unit. The Dzyaloshinskii-Moriya interaction can lead to the canting of the magnetic moments and the appearance of macroscopic magnetization, which causes the polar distortion in BFO . In the BFO-based films with suppressed spiral spin structures, the orientation of spin vectors is coupled with ferroelectric polarization vectors through the ferroelastic strain. When a magnetic field is applied to the BFO-based films, the recanting of the magnetic moments happens, which facilitates the antiferromagnetic domain switching and reduces the activation energy for the switching of the electrical polarization domains . This further gives rise to a change in the ferroelectric domain switching behaviors, causing the variation of ferroelectric polarization under external magnetic fields. In addition, during the magnetoelectric coupling measurements, the leakage current can also affect the observed polarization value under external magnetic fields. In fact, since the background leakage current is inevitably superimposed on the polarization current, the observed polarization value under external magnetic fields is slightly larger than the actual values.
Local Electric Conduction Characteristics Under External Magnetic Fields
We consider that such a local electric conduction behavior under external magnetic fields should be closely related to the ferroelectric polarization response to magnetic fields. Before applying a magnetic field, the oxygen vacancies are randomly distributed in the polycrystalline BLFO thin films. These oxygen vacancies are easily trapped or accumulated at the grain boundaries and domain walls . The presence of oxygen vacancies is a main reason for the large leakage current . When applying a magnetic field to the BLFO thin film, due to the existence of local mangetoelectric coupling in BLFO, the switching behaviors of microscopic ferroelectric domains will change, accompanied with the variation of local electric fields. For compensating the discontinuity of local polarization, the accumulated oxygen vacancies will redistribute due to the switching of ferroelectric domains, consequently leading to the change in local conductive behaviors.
In summary, the local magnetoelectric coupling behaviors were systematically investigated in the multiferroic BLFO polycrystalline thin films. The local ferroelectric polarization response to magnetic fields confirmed the robust existence of local magnetoelectric coupling, and a so-called optimized magnetic field of ~40 Oe was obtained, at which it exhibited the strongest magnetoelectric coupling effect. The further magnetic-field-dependent local conductivity tests showed a local magnetoresistance effect in the film, which could be attributed to the redistribution of bound oxygen vacancies dominated by the polarization-dependent local ferroelectric domain switching under external magnetic fields. This work provides a useful technique to characterize the local magnetoelectric coupling in multiferroic materials and is also beneficial for studying the intrinsic coupling of multiple ferroic orders in BiFeO3-based systems.
This work was supported by the National Key Projects for Basic Research of China (Grant No. 2015CB921203), the National Key Research Programme of China (Grant No. 2016YFA0201004), the National Natural Science Foundation of China (Grant Nos. 51472113 and 11134005).
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Eerenstein W, Mathur ND, Scott JF (2006) Multiferroic and magnetoelectric materials. Nature 442:759–765View ArticleGoogle Scholar
- Ramesh R, Spaldin NA (2007) Multiferroics: progress and prospects in thin films. Nat Mater 6:21–29View ArticleGoogle Scholar
- Nan CW, Bichurin MI, Dong SX, Viehland D, Srinivasan G (2008) Multiferroic magnetoelectric composites: historical perspective, status, and future directions. J Appl Phys 103:031101View ArticleGoogle Scholar
- Vaz CAF, Hoffman J, Ahn CH, Ramesh R (2010) Magnetoelectric coupling effects in multiferroic complex oxide composite structures. Adv Mater 22:2900–2918View ArticleGoogle Scholar
- Ma J, Hu JM, Li Z, Nan CW (2011) Recent progress in multiferroic magnetoelectric composites: from bulk to thin films. Adv Mater 23:1062–1087View ArticleGoogle Scholar
- Hur N, Park S, Sharma PA, Ahn JS, Guha S, Cheong SW (2004) Electric polarization reversal and memory in a multiferroic material induced by magnetic fields. Nature 429:392–395View ArticleGoogle Scholar
- Lottermoser T, Lonkai T, Amann U, Hohlwein D, Ihringer J, Fiebig M (2004) Magnetic phase control by an electric field. Nature 430:541–544View ArticleGoogle Scholar
- Li LJ, Li JY, Shu YC, Yen JH (2008) The magnetoelectric domains and cross-field switching in multiferroic BiFeO3. Appl Phys Lett 93:192506View ArticleGoogle Scholar
- Ravindran P, Vidya R, Kjekshus A, Fjellvag H, Eriksson O (2006) Theoretical investigation of magnetoelectric behavior in BiFeO3. Phys Rev B 74:224412View ArticleGoogle Scholar
- Catalan G, Scott JF (2009) Physics and applications of bismuth ferrite. Adv Mater 21:2463–2485View ArticleGoogle Scholar
- Singh SK, Ishiwara H (2006) Doping effect of rare-earth ions on electrical properties of BiFeO3 thin films fabricated by chemical solution deposition. Jpn J Appl Phys 45:3194–3197View ArticleGoogle Scholar
- Kawae T, Terauchi Y, Tsuda H, Kumeda M, Morimoto A (2009) Improved leakage and ferroelectric properties of Mn and Ti codoped BiFeO3 thin films. Appl Phys Lett 94:112904View ArticleGoogle Scholar
- Kim JK, Kim SS, Kim WJ, Bhalla AS, Guo RY (2006) Enhanced ferroelectric properties of Cr-doped BiFeO3 thin films grown by chemical solution deposition. Appl Phys Lett 88:132901View ArticleGoogle Scholar
- Wang Y, Nan CW (2006) Enhanced ferroelectricity in Ti-doped multiferroic BiFeO3 thin films. Appl Phys Lett 89:052903View ArticleGoogle Scholar
- Lazenka VV, Ravinski AF, Makoed II, Vanacken J, Zhang G, Moshchalkov VV (2012) Weak ferromagnetism in La-doped BiFeO3 multiferroic thin films. J Appl Phys 111:123916View ArticleGoogle Scholar
- Solovyev IV, Pchelkina ZV (2010) Magnetic-field control of the electric polarization in BiMnO3. Phys Rev B 82:094425View ArticleGoogle Scholar
- Wang F, Zou T, Yan LQ, Liu Y, Sun Y (2012) Low magnetic field reversal of electric polarization in a Y-type hexaferrite. Appl Phys Lett 100:122901View ArticleGoogle Scholar
- Xie SH, Liu YM, Liu XY, Zhou QF, Shung KK, Zhou YC, Li JY (2010) Local two-way magnetoelectric couplings in multiferroic composites via scanning probe microscopy. J Appl Phys 108:054108View ArticleGoogle Scholar
- Chung TK, Carman GP, Mohanchandra KP (2008) Reversible magnetic domain-wall motion under an electric field in a magnetoelectric thin film. Appl Phys Lett 92:112509View ArticleGoogle Scholar
- Chung TK, Keller S, Carman GP (2009) Electric-field-induced reversible magnetic single-domain evolution in a magnetoelectric thin film. Appl Phys Lett 94:132501View ArticleGoogle Scholar
- Guo YP, Guo B, Dong W, Li H, Liu HZ (2013) Evidence for oxygen vacancy or ferroelectric polarization induced switchable diode and photovoltaic effects in BiFeO3 based thin films. Nanotechnology 24:275201View ArticleGoogle Scholar
- Li ZG, Chen TS, Pan HY, Song FQ, Wang BG, Han JH, Qin YY, Wang XF, Zhang R, Wan JG, Xing DY, Wang GH (2012) Two-dimensional universal conductance fluctuations and the electron-phonon interaction of surface states in Bi2Te2Se microflakes. Sci Rep 2:595Google Scholar
- Ederer C, Spaldin NA (2005) Weak ferromagnetism and magnetoelectric coupling in bismuth ferrite. Phys Rev B 71:060401View ArticleGoogle Scholar
- Zhou MX, Chen B, Sun HB, Wan JG, Li ZW, Liu JM, Song FQ, Wang GH (2013) Local electrical conduction in polycrystalline La-doped BiFeO3 thin films. Nanotechnology 24:225702View ArticleGoogle Scholar
- Caruntu G, Yourdkhani A, Vopsaroiu M, Srinivasan G (2012) Probing the local strain-mediated magnetoelectric coupling in multiferroic nanocomposites by magnetic field-assisted piezoresponse force microscopy. Nanoscale 4:3218–3227View ArticleGoogle Scholar
- Wang J, Neaton JB, Zheng H, Nagarajan V, Ogale SB, Liu B, Viehland D, Vaithyanathan V, Schlom DG, Waghmare UV, Spaldin NA, Rabe KM, Wuttig M, Ramesh R (2003) Epitaxial BiFeO3 multiferroic thin film heterostructures. Science 299:1719–1722View ArticleGoogle Scholar
- Baettig P, Ederer C, Spaldin NA (2005) First principles study of the multiferroics BiFeO3, Bi2FeCrO6, and BiCrO3: structure, polarization, and magnetic ordering temperature. Phys Rev B 72:214105View ArticleGoogle Scholar
- Cheng ZX, Wang XL (2007) Room temperature magnetic-field manipulation of electrical polarization in multiferroic thin film composite BiFeO3/La2/3Ca1/3MnO3. Phys Rev B 75:172406View ArticleGoogle Scholar
- Stojadinovic B, Vasic B, Stepanenko D, Tadic N, Gajic R, Dohcevic-Mitrovic Z (2016) Variation of electric properties across the grain boundaries in BiFeO3 film. J Phys D Appl Phys 49:045309View ArticleGoogle Scholar
- Seidel J, Maksymovych P, Batra Y, Katan A, Yang SY, He Q, Baddorf AP, Kalinin SV, Yang CH, Yang JC, Chu YH, Salje EKH, Wormeester H, Salmeron M, Ramesh R (2010) Domain wall conductivity in La-doped BiFeO3. Phys Rev Lett 105:197603View ArticleGoogle Scholar
- Shen W, Bell A, Karimi S, Reaney IM (2012) Local resistive switching of Nd doped BiFeO3 thin films. Appl Phys Lett 100:133505View ArticleGoogle Scholar